Thermally promoted addition of undecylenic acid on thermally hydrocarbonized porous silicon optical reflectors
© Jalkanen et al.; licensee Springer. 2012
Received: 5 April 2012
Accepted: 30 May 2012
Published: 19 June 2012
Thermally promoted addition of undecylenic acid is studied as a method for modifying porous silicon optical reflectors that have been pre-treated with thermal hydrocarbonization. Successful derivatization of undecylenic acid is demonstrated and confirmed with Fourier transform infrared and X-ray photoelectron spectroscopies. The results indicate that the hydrocarbonization pre-treatment considerably improves stability against oxidation and chemical dissolution in basic environments. The two-step treatment also does not cause an appreciable change on sample reflectance spectra, which enables the use of the functionalized structures in optical sensing applications.
KeywordsPorous silicon Interference filter Optical microcavity Chemical stability
The use of nanostructured porous silicon (PSi) in biosensing applications has received a lot of attention in recent years [1–5]. This interest is, for the most part, due to the large internal surface area and easily functionalizable surface of PSi . In addition, fabrication of PSi with electrochemical anodization is a straightforward process that enables control over the pore size and morphology of the resulting material. The favorable optical properties of PSi also enable the preparation of interference filters and optical thin films . Furthermore, PSi-based thin films and optical filters have been used in gas and biosensing applications [8, 9]. We also need to mention 1/f noise in polymorphous silicon films [10, 11].
The surface of freshly prepared PSi is covered with hydride species and can therefore be functionalized by grafting molecules, with functional groups, on the surface [12, 13]. This can be achieved, for example, with thermal hydrosilylation of undecylenic acid . Even though the stability of modified PSi in basic solutions, such as aqueous KOH, is considerably increased, the surface coverage is not complete, and hydrides remain on the surface [15, 16]. These un-reacted Si-H bonds on PSi surface are susceptible to oxidation, and furthermore, oxidized surface slowly dissolves in aqueous basic solutions [2, 17]. This phenomenon has been linked with baseline drift of PSi-based biosensors, leading to non-reproducible results . More complete surface passivation may be obtained with the thermal hydrocarbonization (THC) treatment . Moreover, the utilization of THC-treated PSi optical filters, in gas sensing applications, has already been demonstrated . Lately, it has also been shown that the THCPSi surface may also be further functionalized by attaching molecules with a functional group to the hydrocarbonized surface [20, 21].
In this work, we evaluate the effects of thermally promoted undecylenic acid addition on THCPSi optical reflectors. Successful functionalization of the hydrocarbonized surface is verified with Fourier transform infrared (FTIR) and X-ray photoelectron spectroscopies (XPS). The stability of the modified THCPSi surface is tested under several high-pH environments and compared to as-anodized PSi and PSi treated with thermal hydrosilylation of undecylenic acid. A large improvement in the stability is observed, which indicates that the new two-step treatment is promising for producing optical biosensors.
Porous silicon-based optical microcavities and rugate filters were prepared by anodizing single-crystal boron-doped p-type Si wafers ((100) 0.005 to 0.03 Ω cm) in an electrolyte solution composed of HF (46-48 wt.%) and ethanol in 1:1.7 ratio (v/v). The anodization current was controlled with a programmable current source (Keithley 6221, Keithley Instruments Inc., Cleveland, OH, USA). Sinusoidal anodization current with current density values oscillating between 63.3 and 113.9 mA/cm2 was used. The sine wave period length was 5 s, and the total anodization time was 210 s. A cavity layer was added in the middle by applying 63.3 mA/cm2 of constant current density for 12.5 s. Samples were prepared in a single-tank electrochemical cell, which left an area of 0.79 cm2 of the Si electrode exposed to the electrolyte. InGa eutectic was applied to the backside of the Si electrodes to ensure an ohmic contact with the Cu plate, which was used as a current collector. Prior to the anodization, the Si samples were cleaned with successive ultrasonic treatments in acetone and ultrapure water (Millipore, Milli-Q Gradient, Millipore Co., Billerica, MA, USA) and finally dipped in HF (5 wt.%) to remove surface oxides.
Thermal hydrocarbonization was performed on dried samples in a quartz tube . After a 15-min acetylene treatment at 500°C, the samples were cooled down to room temperature under nitrogen flow. The hydrocarbonized porous Si samples were immersed in neat undecylenic acid solution for 16 h at 120°C, which resulted in partial carboxyl group termination .
Derivatization of undecylenic acid was also performed on as-anodized PSi. After anodization, the dried samples were inserted into a round bottom flask and immersed in neat undecylenic acid solution. The flask was then connected to a Schlenk line and purged with three vacuum-refill cycles. The samples were treated under argon atmosphere for 20 h at 120°C. After both treatments, the functionalized samples were copiously rinsed with dichloromethane, tetrahydrofuran, and ethanol to remove excess undecylenic acid.
Reflectance measurements were conducted with an Ocean Optics HR4000CG-UV-NIR spectrometer (Ocean Optics, Inc., FL, USA), which was connected to a tungsten halogen lamp (LS-1, Ocean Optics). FTIR spectra were recorded with a Perkin Elmer Spectrum BX spectrometer (PerkinElmer, Waltham, MA, USA) using an attenuated total reflectance (ATR) accessory (MIRacle, Pike Technologies Inc., Madison, WI, USA). Microcavity structure was examined with scanning electron microscopy (JEOL JSM-6500FE, JEOL Ltd., Akishima, Tokyo, Japan). XPS (JEOL JPS-9010MC) was used for analyzing the surface of the chemically modified microcavities. Al K α line (1,486.6 eV) was used as an X-ray source and operated at 10 kV and 10 mA (100 W). The samples were kept in high vacuum up to 10-7 Pa during the XPS measurements. Binding energies were referenced to adventitious carbon C 1s signal at 284.5 eV. Thermogravimetric measurements (TGA 7, Perkin Elmer) were used for assessing the thermal stability of the samples.
Methylamine (MA) (mixed in water, 40%) vapor measurements were conducted in an atmospheric chamber equipped with an optical window. Vapor concentration inside the chamber was controlled by adjusting relative gas-flow ratios with mass-flow controllers. Nitrogen was used as carrier gas . Gas-liquid chromatography (GLC) (GC-14B, Shimadzu Corporation, Nakagyo-ku, Kyoto, Japan) was used for determining the MA concentration. Concentration was determined by directing the gas stream (nitrogen and MA) inside 20 mL of 1.0 M HCl aqueous solution for 1 min. Phenolphthalein solution (0.1%; approximately 90% ethanol, 200 μ L) and isopropanol (internal reference, 42.0 μ L, 0.500 mmol) were added to the solution. Back titration was performed with NaOH (1.0 M) aqueous solution and was used for confirming the results. NaOH solution was added slightly in excess (ca 21 mL), and the solution was analyzed with GLC.
Results and discussion
Changes in the chemical composition
The gradual change in the surface chemistry of the PSi structure during the UnTHC treatment is clearly seen in the FTIR spectra (Figure 1). Spectrum recorded for the as-anodized sample displays peaks related to stretching of hydride species at 2,100 cm-1. Peaks caused by SiH2 scissor bending and wagging are observed at 916 and 628 cm-1, respectively . SiH bending at 667 cm-1 is also visible . After thermal hydrocarbonization, these peaks disappear and are replaced with strong peaks around 1,000 cm-1 arising from the hydrocarbon termination . In addition, smaller peaks related to hydrocarbon species are observed at 2,950 cm-1. As the hydrocarbon surface is functionalized with undecylenic acid, emergence of three new peaks is clearly observed (Figure 1). Peaks due to the stretching and deformation of CH2 of the alkyl chain appear at 2,922 and 1,460 cm-1, respectively . The absorption peak at 1,712 cm-1 is attributed to the carbonyl stretching (ν CO) and indicates a partial carboxyl termination of the UnTHC-treated surface. Comparison between the FTIR spectra recorded for the UnTHCPSi and UnPSi-treated microcavities shows that the peaks related to successful addition of undecylenic acid on the surface appear exactly at same wavenumber regions for both samples (Figure 2). Although the exact chemical reaction mechanism is not clear, thermogravimetry measurements clearly show the strong thermal stability of UnTHCPSi and rule out the possibility of mere physisorption [see Figure S1 in Additional file 1.
The differences in chemical composition are also clearly seen in the XPS survey spectra recorded for as-anodized PSi, UnPSi, and UnTHCPSi microcavities (Figure 3). As-anodized PSi shows clear peaks for Si, whereas only trace amounts of C, F, and O are observed (Figure 3a). An increase in carbon and oxygen contents can be observed in the spectra recorded for UnPSi and UnTHCPSi (Figure 3b,c, respectively). This is seen as strengthening of the C 1s and O 1s peaks as well as the appearance of Auger peaks. The C 1s core level spectra also reveal a small peak at an approximate binding energy of 289.5 eV, which is characteristic to the carboxyl group [14, 23].
Effects of chemical modification on PSi optical reflectors
Effects of the chemical modifications on the reflectance spectra of PSi microcavities are shown in Figure 4. Both treatments, namely thermal hydrosilylation of undecylenic acid (UnPSi) and thermally promoted addition of undecylenic acid on thermally hydrocarbonized porous silicon (UnTHCPSi), resulted in a shift of the reflectance spectrum. The UnPSi spectra showed a redshift that was usually in the order of 20 to 38 nm (Figure 4a), whereas the UnTHC treatment usually resulted in a redshift in the order of 1 to 10 nm (Figure 4b). The exact value of the spectral shift varied between samples for both chemical modifications, indicating that the amount of undecylenic acid bound on the surface is quite sensitive to slight changes in experimental conditions. The redshift recorded for the UnPSi is related to the covalent attachment of the undecylenic acid molecule on the inner surface of the porous structure. The UnTHC treatment is a two-step process where the thermal hydrocarbonization causes a blueshift in the order of 10 nm followed by a successive redshift as the undecylenic acid binds to the THCPSi surface .
The shape of the reflectance spectra remains virtually unchanged for both UnPSi and UnTHCPSi microcavities (Figure 4). Moreover, the quality of the cavity resonance, which is very delicate to slight changes in the structure, was not affected. The best FWHM values recorded for the cavities were smaller than 2.5 nm (Figure 4c). Figure 5 shows a cross-sectional scanning electron micrograph of an UnTHC-modified PSi microcavity. It is obvious that the cavity structure is preserved after the treatment, and well-defined interfaces can be observed between the cavity layer and the upper and lower filter layers (Figure 5b).
Stability under basic environments
As-anodized PSi is highly unstable under basic conditions. This is demonstrated in Figure 6, where a clear blueshift in the reflectance spectrum of a PSi rugate filter is observed after just 5-min exposure to 10.7% of MA vapor. Usually when vapor adsorbs inside a PSi optical reflector, a redshift, connected to an increase in the effective refractive index, is observed . However, in this case, the MA vapor creates highly basic conditions inside the porous matrix resulting in rapid oxidation. This is seen as an instantaneous blueshift, which increases in accordance with exposure time (Figure 6b). After 47-min recovery period, an irreversible blueshift close to 30 nm is observed. When the same experiment is performed for a UnPSi rugate filter, the filter displays a redshift upon MA adsorption. A blueshift in the order of 2 nm is observed after the 47-min recovery period, indicating slight oxidation. The UnTHCPSi rugate filter also displays a redshift when exposed to MA vapor, but unlike the as-anodized PSi and UnPSi filters, no blueshift is observed. This suggests that sample stability against oxidation is increased, as discussed in reference .
In order to compare the stability of differently modified surfaces in aqueous solutions, as-anodized PSi, UnPSi, and UnTHCPSi microcavities were immersed in 1 M solutions of aqueous NaOH and KOH. The as-anodized samples dissolved within 30 s in both NaOH and KOH solutions. The UnPSi microcavities displayed considerably improved stability, and complete dissolution was observed after 2.5 min. Unlike the as-anodized microcavities and microcavities treated with thermal hydrosilylation of undecylenic acid, the UnTHC-treated microcavities did not display prominent bubble formation upon immersion to NaOH or KOH. Figure 7 shows the reflectance spectra measured for freshly prepared UnPSi and UnTHCPSi microcavities and the spectra after immersion to aqueous NaOH (Figure 7a) and KOH (Figure 7b). The spectra for UnPSi cavities show clear dissolution after only 1-min immersion. In stark contrast, the spectra measured for UnTHC cavities show only minor changes even after 1-h immersion to NaOH and 2-h immersion to KOH. Moreover, the position of the cavity resonance has remained virtually unchanged. Based on the stability exhibited by UnTHCPSi optical reflectors and also taking into account the possibility for further surface functionalization of the UnTHCPSi structure [see Figure S2 in Additional file 1], we can conclude that the UnTHCPSi reflectors show promise for utilization in biosensing applications.
After 24 h of immersion, the UnTHC-treated microcavity had completely dissolved in KOH. The sample immersed in NaOH had still not completely dissolved, but the porous layer had become detached from the substrate, and broke into fragments as we tried to remove it from the beaker. The slight differences observed for dissolution in NaOH and KOH are attributed to experimental error. Immersion times required for complete dissolution of differently modified microcavities are gathered in Table 1.
Immersion time needed for dissolving PSi microcavities in aqueous solutions
1 M NaOH
1 M KOH
Undecylenic acid addition to thermally hydrocarbonized PSi was demonstrated. The incorporation of the molecule on the THCPSi surface was verified with FTIR and XPS measurements. In addition, UnTHC treatment has only minor effects on the optical quality of PSi-based interference reflectors, and even delicate structures such as optical microcavities can be modified with the UnTHC treatment. UnTHCPSi showed remarkable improvement in stability when compared to as-anodized PSi and UnPSi. The improved stability under aqueous basic solutions suggests that the functionalized surface would be useful in developing optical biosensors.
This work was partially supported by the Grant-in-Aid from the Japan Society of Promotion of Science for Scientific Research (B) under grant number 22350092. The authors would like to thank Dr. Y.-I. Suzuki from C. Uyemura & Co. Ltd. for technical assistance with the XPS measurements and Assist. Prof. M. Wakioka and Prof. F. Ozawa from Kyoto University for assistance with GLC measurements. Ms. T. Urata and Mr. R. Koda are acknowledged for helping out with some of the experiments. T. Jalkanen acknowledges financial support from MEXT, the Japanese Ministry of Education, Culture, Sports, Science & Technology.
- Lin VSY, Motesharei K, Dancil KPS, Sailor MJ, Ghadiri MR: A porous silicon-based optical interferometric biosensor. Science 1997, 278: 840–843. 10.1126/science.278.5339.840View Article
- Janshoff A, Dancil KPS, Steinem C, Greiner DP, Lin VSY, Gurtner C, Motesharei K, Sailor MJ, Ghadiri MR: Macroporous p-type silicon Fabry-Perot layers. Fabrication, characterization, and applications in biosensing. J Am Chem Soc 1998, 120: 12108–12116. 10.1021/ja9826237View Article
- Chan S, Fauchet PM, Li Y, Rothberg LJ, Miller BL: Porous silicon microcavities in biosensing applications. Phys Status Solidi A 2000, 182: 541–546. 10.1002/1521-396X(200011)182:1<541::AID-PSSA541>3.0.CO;2-#View Article
- Chan S, Horner SR, Fauchet PM, Miller BL: Identification of gram negative bacteria using nanoscale silicon microcavities. J Am Chem Soc 2001, 123: 11797–11798. 10.1021/ja016555rView Article
- Jane A, Dronov R, Hodges A, Voelcker NH: Porous silicon biosensors on the advance. Trends Biotechnol 2009, 27: 230–239. 10.1016/j.tibtech.2008.12.004View Article
- Salonen J, Lehto VP: Fabrication and chemical surface modification of mesoporous silicon for biomedical applications. Chem Eng J 2008, 137: 162–172. 10.1016/j.cej.2007.09.001View Article
- Torres-Costa V, Martín-Palma RJ: Application of nanostructured porous silicon in the field of optics. A review. J Mater Sci 2010, 45: 2823–2838. 10.1007/s10853-010-4251-8View Article
- Snow PA, Squire EK, Russell PSJ, Canham L: Vapor sensing using the optical properties of porous silicon Bragg mirrors. J Appl Phys 1999, 86: 1781–1784. 10.1063/1.370968View Article
- Pacholski C, Sartor M, Sailor MJ, Cunin F, Miskelly GM: Biosensing using porous silicon double-layer interferometers: reflective interferometric Fourier transform spectroscopy. J Am Chem Soc 2005, 127: 11636–11645. 10.1021/ja0511671View Article
- Li SB, Wu ZM, Jiang YD, Li W, Liao NM, Yu JS: Structure and 1/f noise of boron doped polymorphous silicon films. Nanotechnology 2008, 19: 085706. 10.1088/0957-4484/19/8/085706View Article
- Li S, Jiang Y, Wu Z, Wu J, Ying Z, Wang Z, Li W, Salamo G: Origins of 1/f noise in nanostructure inclusion polymorphous silicon films. Nanoscale Res Lett 2011, 6: 281. 10.1186/1556-276X-6-281View Article
- Buriak JM: Silicon-carbon bonds on porous silicon surfaces. Adv Mater 1999, 11: 265–267. 10.1002/(SICI)1521-4095(199903)11:3<265::AID-ADMA265>3.0.CO;2-WView Article
- Stewart MP, Buriak JM: Chemical and biological applications of porous silicon technology. Adv Mater 2000, 12: 859–869. 10.1002/1521-4095(200006)12:12<859::AID-ADMA859>3.0.CO;2-0View Article
- Boukherroub R, Wojtyk JT, Wayner DDM, Lockwood DJ: Thermal hydrosilylation of undecylenic acid with porous silicon. J Electrochem Soc 2002, 149: H59-H63. 10.1149/1.1432679View Article
- Buriak JM, Allen MJ: Lewis acid mediated functionalization of porous silicon with substituted alkenes and alkynes. J Am Chem Soc 1998, 120: 1339–1340. 10.1021/ja9740125View Article
- Lees IN, Lin H, Canaria CA, Gurtner C, Sailor MJ, Miskelly GM: Chemical stability of porous silicon surfaces electrochemically modified with functional alkyl species. Langmuir 2003, 19: 9812–9817. 10.1021/la035197yView Article
- Dancil KPS, Greiner DP, Sailor MJ: A porous silicon optical biosensor: detection of reversible binding of IgG to a protein A-modified surface. J Am Chem Soc 1999, 121: 7925–7930. 10.1021/ja991421nView Article
- Salonen J, Björkqvist M, Laine E, Niinistö L: Stabilization of porous silicon surface by thermal decomposition of acetylene. Appl Surf Sci 2004, 225: 389–394. 10.1016/j.apsusc.2003.10.028View Article
- Jalkanen T, Torres-Costa V, Salonen J, Björkqvist M, Mäkilä E, Martínez-Duart JM, Lehto VP: Optical gas sensing properties of thermally hydrocarbonized porous silicon Bragg reflectors. Opt Express 2009, 17: 5446–5456. 10.1364/OE.17.005446View Article
- Sciacca B, Alvarez SD, Geobaldo F, Sailor MJ: Bioconjugate functionalization of thermally carbonized porous silicon using a radical coupling reaction. Dalton T 2010, 39: 10847–10853. 10.1039/c0dt00936aView Article
- Kovalainen M, Mönkäre J, Mäkilä E, Salonen J, Lehto VP, Herzig KH, Järvinen K: Mesoporous silicon (PSi) for sustained peptide delivery: effect of PSi microparticle surface chemistry on peptide YY3–36 release. Pharm Res 2012, 29: 837–846. 10.1007/s11095-011-0611-6View Article
- Ogata YH, Niki H, Sakka T, Iwasaki M: Hydrogen in porous silicon: vibrational analysis of SiHx species. J Electrochem Soc 1995, 142: 195–201. 10.1149/1.2043865View Article
- Jalkanen T, Mäkilä E, Suzuki YI, Urata T, Fukami K, Sakka T, Salonen J, Ogata YH: Studies on chemical modification of porous silicon-based graded-index optical microcavities for improved stability under alkaline conditions. Adv Funct Mater 2012. 10.1002/adfm.201200386 10.1002/adfm.201200386
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.